* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project
179 PLASTICS IN FOOD PACKAGING Plastic granules External electrical heating elements Die Motor Molten plastic Figure 7.1 Extruder. conversion of plastic resin into films, sheets, containers etc., is to change the pellets from solid to liquid or molten phase in an extruder. The plastic is melted by a combination of high pressure, friction and externally applied heat. This is done by forcing the pellets along the barrel of an extruder using specially designed, polymer-specific, screw under controlled conditions that ensure the production of a homogeneous melt prior to extrusion (Fig. 7.1). In the manufacture of film and sheet, the molten plastic is then forced through a narrow slot or die. In the manufacture of rigid packaging, such as bottles and closures, the molten plastic is forced into shape using a precisely machined mould. 7.2.2 Plastic film and sheet for packaging Generally, films are by definition less than 100 Î¼m thick (1 micron is 0.000001 metres or 1 Ã 10â6 m). Film is used to wrap product, to overwrap packaging (single packs, groups of packs, palletised loads), to make sachets, bags and pouches, and is combined with other plastics and other materials in laminates, which in turn are converted into packaging. Plastic sheets in thicknesses up to 200 Î¼m are used to produce semi-rigid packaging such as pots, tubs and trays. The properties of plastic films and sheets are dependent on the plastic(s) used and the method of film manufacture together with any coating or lamination. In film and sheet manufacture, there are two distinct methods of processing the molten plastic which is extruded from the extruder die. In the cast film process, the molten plastic is extruded through a straight slot die onto a cooled cylinder, known as the chill roll (Fig. 7.2). In the blown, or tubular, film process, the molten plastic is continuously extruded through a die in the form of a circular annulus, so that it emerges as a tube. The tube is prevented from collapsing by maintaining air pressure inside the tube or bubble (Fig. 7.3). In both the processes, the molten polymer is quickly chilled and solidified to produce a film which is reeled and slit to size.